Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

An analytical solution for the load distribution along a fibre in a nonwoven

network

Warren Batchelor

Australian Pulp and Paper Institute, Department of Chemical Engineering, PO Box

36, Monash University, 3800 Victoria Australia

Email: warren.batchelor@eng.monash.edu.au

+61 3 9905 3452/ Fax: +61 3 9905 3413

Abstract

This paper develops a method to analyse the load distribution along a half fibre in a

non-woven or fibre composite where force is transferred into the fibre at any set of

discrete contacts. The force transferred at each contact is assumed to be proportional

to the displacement of the contact relative to the applied strain field. The constant of

proportionality between displacement and force can be set independently for each

contact. The cross-sectional area and elastic modulus of each segment between

contacts can also be set independently. It was shown that the displacement, due to the

applied strain, at each contact could be expressed in terms of the displacement at the

last contact at the end of the fibre. As the displacement at the last contact was the sum

of the previous contacts, each multiplied by a stress transfer coefficient, the stress

distribution along the fibre could be solved analytically. The debonding of fibres

from a paper sheet under load was simulated. The fibre load-network strain curve was

found to be highly sensitive to the configuration of the crossing points. The method

of analysis has application to nonwoven networks such as paper as well as nonwoven

fibre composites.

Keywords

Short-fibre composites; Mechanical properties; Modelling; Stress transfer; shear-lag

model; Cellulosic fibres

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

Introduction

An important factor affecting the mechanical properties of a fibre network or fibre

composite under load is the stress distribution along fibres in the material. This has

been frequently modelled using the shear-lag theory (Nairn, 1997), due originally to

Cox (Cox, 1952). The shear-lag analysis starts by considering a fibre embedded in a

matrix subject to a strain,

ε

Ⱐ楮⁴桥楲散瑩潮映瑨攠晩扲攮,⁉琠楳獳畭e搠瑨慴⁴桥潡搬d

dF

transferred into the fibre from the matrix, over a distance, dx, at a position, x,

along the fibre is linearly proportional to the displacement of x relative to the applied

strain or

/( )

f

m

dF dx

δ

δ∝ − where

f

δ

湤=

m

δ

are the fibre and network

displacement, respectively, relative to a reference point. For a linearly elastic fibre

this expression can be integrated (Cox, 1952; Raisanen et al., 1997) to give

(

) ( )

( )

( ) 1 cosh/cosh

f

x

x L

ε ε β β= −

, where

(

)

f

x

ε

is the strain at a position

x

along

a fibre of half length,

L

, elastic modulus,

E

and cross-section,

A

, and

β

猠瑨攠獨敡爭

污朠灡lame瑥爠杩≥i湧⁴桥=fi捩敮捹≥⁷桩捨⁴桥a瑲楸⁴牡湳f敲猠獴牥獳s瑯⁴桥i扲攮†

周攠捯潲摩θa瑥祳≥敭猠獥琠睩瑨=

0

x

=

at the centre of the fibre.

The shear-lag model has found widespread application (see for example (Sridhar et

al., 2003; Xia et al., 2002)) in research on fibre reinforced composites. It has also

been used to predict the elastic modulus (Astrom et al., 1994; Page and Seth, 1980)

and strength (Carlsson and Lindstrom, 2005; Feldman et al., 1996) of nonwoven

fibrous networks, such as paper, although the usefulness of the approach has been

disputed (Raisanen et al., 1997). Methods to calculate

β

潲楶敮a瑲楸a瑥物慬≥

慮搠晩扲攠摩ae湳楯湳慶攠扥敮⁴桥畢橥n 琠潦潮瑩湵敤敳敡牣栠⡎慩牮Ⱐㄹ㤷⤮†≥

䡯睥癥爬桥慲慧⁴祰e湡汹=楳猠 潮汹畬汹⁶慬楤映潮攠獩湧汥⁶慬略映

β

灰汩=猠

慬潮朠瑨攠a桯汥敮杴栠潦⁴桥楢牥⸠⁉琠楳h 慬獯楫敬礠瑯攠愠a 潯搠慰灲潸業a瑩潮映瑨攠

癡物慴楯渠楮∝

β

猠獭慬氮†周敲攠慲攠aa湹楴畡瑩潮猠睨敲攠愠獩湧汥⁶慬l攠潦e

β

慮湯琠

扥灰汩敤⸠⁐慰敲Ⱐ景爠數慭灬攬猠 愠湯湷潶敮整睯牫潭灯獥搠潦慴畲慬汹a

灲潤畣敤楢牥猠睩瑨⁷楤攠摩獴物扵瑩潮猠潦 敮杴桳Ⱐ捲潳猭獥捴楯湡氠摩=e湳楯湳湤n

m散桡湩捡氠灲潰敲瑩敳⸠⁌潡搠楳湬e⁴牡湳晥= 牥搠楮瑯楢牥琠摩獣牥瑥⁰潩湴猬⁷桥牥±

瑨攠晩扲攠捯me猠楮瑯潮瑡捴⁷楴栠潴se爠晩扲 敳⸠䙯爠愠杩癥渠晩±±攬慣栠捲潳獩湧楢牥鉳s

摩de湳楯湳Ⱐn散桡湩捡氠灲潰敲瑩敳Ⱐeo獩瑩潮湤±潳獩湧湧l攠睩汬攠ee瑥牭楮敤i

慣捯牤楮朠瑯瑯捨慳瑩挠=i獴物扵瑩潮献† 䄠湯渭睯癥渠潲⁷潶敮楢牥潭p潳楴攠楳o

慮潴桥爠數慭灬攬猠瑨攠獴牥獳 ⁴牡湳晥牲敤湴漠愠晩扲攠潦= 楮瑥牥獴⁷楬氠癡特汯湧⁴桥i

晩扲攬略⁴漠瑨攠摩晦敲敮琠獴牥fs⁴牡湳= 敲桡牡捴敲楳瑩捳映瑨攠晩扲攠湥瑷潲e湤=

ma瑲楸⸠⁆楮慬汹湹ib±攠湥瑷潲欠潲i扲攠捯bp潳楴攠⡥朠捥汬l汯獩挠捯lp潳楴敳a摥d

潦污砠潲潴瑯渠晩扲敳
䕩捨桯牮湤⁙ 潵湧Ⱐ㈰〳⤩渠睨楣栠獴牥獳猠瑲慮獦敲牥搠

慣牯獳⁴桥湤猠潦⁴桥楢牥猠睩汬汳漠湯琠 晵汦楬⁴桥污獳楣桥慲慧物瑥物潮Ⱐ慬瑨潵杨f

獯se⁴桥潲整楣慬灰牯慣桥猠桡癥敥渠摥 癥汯灥搠瑯敡氠睩瑨畣栠捡獥猠⡃汹湥Ⱐ

ㄹ㠹⤮1

=

周攠獴牥獳ⵤ楳瑲楢畴楯渠慬潮朠愠晩扲攠桡猠湥癥 爠扥敮潬癥搠慮慬祴楣慬汹潲整睯牫±

睨敲攠汯慤猠瑲慮獦敲牥w湴= 楢牥琠獯=e整映摩獣 牥瑥潮瑡捴⁰±楮瑳Ⱐ敡捨⁷楴栠

慮湤楶楤畡氠癡汵攠潦a

β

Ⱐ慬瑨潵杨琠楳⁰潳獩扬攠瑯,汣畬慴攠畳楮朠晩湩瑥汥浥湴l

浯摥汳⸠⁔桥⁰牯扬敭猠摩晦楣畬琠瑯湡汹= 攠e散慵獥湹潲捥⁴牡湳晥牲敤湴漠瑨攠

晩扲攠扯瑨⁰牯摵捥猠慮搠楳慵獥搠批楳灬f 捥′敮琠瑨攠捯湴慣琠灯楮琠慬潮朠瑨攠晩扲攬e

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

relative to the applied strain. The purpose of this paper is to present an analytical

method to solve this problem.

Theory

Figure 1 shows half of a fibre, which is connected to an external fibre network by

i

contact points. The contact points are shown in Figure 1 as fibres. This is for

convenience and in fact the analysis is valid for any form of stress transfer into the

fibre that is linearly coupled to the network strain in the direction of the fibre.

The fibre is assumed to be linear elastic. The centre of the fibre at

0

0x =

is set as the

reference point and it is assumed that the force transferred into each half of the fibre is

identical and so therefore only half the fibre needs to be considered for the purposes

of this calculation. A strain of

ε

猠慰灬楥搠瑯⁴桥硴敲p慬a瑷潲欠楮⁴桥楲散瑩潮≥=

瑨攠晩扲攠慸楳⸠⁉琠楳獳ime搠瑨慴潲捥猠 瑲慮獦敲牥搠楮瑯⁴桥楢牥礠摩獰污捥l敮瑳映

瑨攠捯湴慣琠≥o楮瑳牯i⁴桥楲煵i汩扲極l= 灯獩瑩潮潲⁴桥灰汩敤整睯牫瑲慩渮†周攠

摩獰污捥d敮琠潦⁴桥e

j

th

contact is designated

j

δ

. The forces that develop at the

j

th

contact are assumed to linearly related to

j

δ

礠愠獴牥獳⁴牡湳晥爠捯敦晩捩敮琬=

j

β

Ⱐ獵捨,

瑨慴≥

j

j j

F

β

δ

=

(1)

The idea is illustrated in Fig. 2, which shows segment 1 of the loaded fibre from Fig.

1. This has a strain in the first segment of

1

ε

⁷桩捨楦晥牳牯=⁴桥整睯牫瑲慩測=

ε

Ⱐ摩獰污捩湧⁴桥牯獳楮朠灯楮琠晲 潭⁴桥煵楬楢物畭⁰潳楴楯渠批=

( )

( )

1 1 1 0

x

xδ ε ε= − −

. It should be noted here that the values of

δ

牥汷慹猠

湥条瑩n攮†周慴猠瑨攠摩ep污捥l敮琠慴慣栠 灯楮≥映瑨攠捲潳獩湧楢牥猠慬睡祳敳猠

瑨慮⁴桥i獰污捥l敮琠潦⁴桥整睯牫e敬慴楶 攠瑯⁴桥敦敲敮捥⁰潩湴⸠⁈敮捥⁴桥≥牥獳±

瑲慮獦敲潥晦楣楥湴猬≥

β

Ⱐ慲攠慬獯敧a瑩癥漠瑨慴⁴≥攠景牣攠潮⁴e攠晩扲攠楳渠瑨攠

灯獩瑩p攠摩牥捴楯測s湤i捡瑥搮††

=

周攠景牣攠睨楣栠桡猠灲θ摵捥搠瑨攠d≥牡楮±

1

ε

猠瑨攠獵m=⁴桥o牣敳敶±汯le搠慴汬l

i

crossing fibres and therefore

( )

( )

1

1 1

1 1

1

0

0

j i

j j

j

x

x

E A

δ βδ ε

=

=

−

= − −

∑

(2)

where

1

E

and

1

A

are the elastic modulus and cross-sectional area, respectively, of

segment 1. Each segment is assumed to have a constant cross-section and elastic

modulus. However, one of the strengths of the method is that the elastic modulus and

the cross-section can vary from segment to segment.

The displacement at the second contact is the sum of the displacement in the first and

second segments which gives

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

( )

( )

1 2

2 1 2 1

1 1 2 2

0

j i j i

j j j j

j j

x x x

E A E A

βδ βδ

δ

ε ε

= =

= =

⎛ ⎞ ⎛ ⎞

⎜ ⎟ ⎜ ⎟

⎜ ⎟ ⎜ ⎟

= − − + − −

⎜ ⎟ ⎜ ⎟

⎝ ⎠ ⎝ ⎠

∑ ∑

(3)

if

1 1 2 2

E A E A

=

then equation (3) simplifies to

2 1 1 1 2 2

2

1

j i

j j

j

x

x x

EA

δ

βδ βδ ε

=

=

⎛ ⎞

⎜ ⎟

= + −

⎜ ⎟

⎝ ⎠

∑

(4)

It can be shown that for the

1n −

th

and

n

th

contacts that

( )

( )

1 1

1 1

1 1 1 2

1 1 1 1

0....

j i j i

j j n n

j j n

n n n

n n

x x x

E A E A

βδ β δ

δ

ε ε

= =

− −

= = −

− − −

− −

⎛ ⎞ ⎛ ⎞

⎜ ⎟ ⎜ ⎟

⎜ ⎟ ⎜ ⎟

= − − + + − −

⎜ ⎟ ⎜ ⎟

⎝ ⎠

⎝ ⎠

∑ ∑

(5)

and

( )

( )

( )

1 1

1 1

1 1 2 1

1 1 1 1

0....

j i j i j i

j j n n n n

j j n j n

n n n n n

n n n n

x x x x x

E A E A E A

βδ β δ βδ

δ

ε ε ε

= = =

− −

= = − =

− − −

− −

⎛ ⎞ ⎛ ⎞ ⎛ ⎞

⎜ ⎟ ⎜ ⎟ ⎜ ⎟

⎜ ⎟ ⎜ ⎟ ⎜ ⎟

= − − + + − − + − −

⎜ ⎟ ⎜ ⎟ ⎜ ⎟

⎝ ⎠

⎝ ⎠ ⎝ ⎠

∑ ∑ ∑

(6)

Substitution of equation (5) in equation (6) yields

( )

1 1

j i

n n

j n

n n n n

n n

x x

E A

βδ

δ

δ ε

=

=

− −

⎛ ⎞

⎜ ⎟

⎜ ⎟

= + − −

⎜ ⎟

⎝ ⎠

∑

(7)

which may be rewritten as

( )

1 1

j i

n n

j n

n n n n

n n

x x

E A

βδ

δ

δ ε

=

=

− −

⎛ ⎞

⎜ ⎟

⎜ ⎟

= − − −

⎜ ⎟

⎝ ⎠

∑

(8)

Thus

1i

δ

−

, can be written in terms of

i

δ

;

2i

δ

−

can be written in terms of

1i

δ

−

and

thus in terms of

i

δ

, and a similar chain can be developed such that each displacement

can be expressed in terms of

i

δ

, the displacement at the final crossing nearest the

fibre end. The displacements at all the fibre crossings can be expressed in terms of

i

δ

and as

i

δ

is given by

( )

( )

( )

1 1

1 1

1 1 2 1

1 1 1 1

0....

j i j i j i

j j i i i i

j j i j i

i i i i i

i i i i

x x x x x

E A E A E A

βδ β δ βδ

δ

ε ε ε

= = =

− −

= = − =

− − −

− −

⎛ ⎞ ⎛ ⎞ ⎛ ⎞

⎜ ⎟ ⎜ ⎟ ⎜ ⎟

⎜ ⎟ ⎜ ⎟ ⎜ ⎟

= − − + + − − + − −

⎜ ⎟ ⎜ ⎟ ⎜ ⎟

⎝ ⎠

⎝ ⎠ ⎝ ⎠

∑ ∑ ∑

(9)

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

which may be expressed in shortened form as

( )

1

1

j i

k i

k k

i j j i

k k

k j k

x x

x

E A

δ

βδ ε

=

=

−

= =

⎛ ⎞

−

⎜ ⎟

= −

⎜ ⎟

⎝ ⎠

∑ ∑

(10)

then it is possible to solve this equation to determine

i

δ

and thus to uniquely

determine the displacements at all crossings. It is also worth noting that if

EA

is

constant along the length of the fibre, then equation (10) simplifies to

1

1

j i

i j j j i

j

x

x

EA

δ

βδ ε

=

=

⎛ ⎞

⎜ ⎟

= −

⎜ ⎟

⎝ ⎠

∑

(11)

To illustrate the application of the method, the equations will now be given for the

relatively simple case of three points of stress transfer for a half fibre with uniform

elastic modulus,

E

, and cross-sectional area,

A

. To simplify the expressions, the

stress transfer coefficients will be no rmalised by the elastic modulus and cross

sectional area such that

/

j j

EA

β

β

′

= (12)

The three points for stress transfer are designated 1, 2 and 3, with point 3 being

closest to the end of the fibre. From equation (8) it can be shown that

( )

(

)

2 3 3 2 3 3

x x

δ

δ ε βδ

′

= + − +

(13)

and

( )( )

( )

( )( )

(

)

(

)

(

)

1 3 3 2 3 3 2 1 3 3 2 3 3 2 3 3

+x x x x x xδ δ ε βδ ε βδ β δ ε βδ

′ ′ ′ ′

= + − + + − + + − +

(14)

And from equation (11)

3

δ

猠杩癥渠批=

㌱ 1 1 2 2 2 3 3 3 3

x

x x x

δ

βδ βδ βδ ε

′ ′ ′

= + + −

(15)

Which upon substitution of equations (13) and (14) yields

( )( )

( )

( )( )

( )

(

)

(

)

( )

( )( )

( )

1 1 3 3 2 3 3 2 1 3 3 2 3 3 2 3 3

2 2 3 3 2 3 3 3 3 3 3 3

0 +x x x x x x x

x x x x x

β δ ε βδ ε βδ β δ ε βδ

β δ ε βδ βδ ε δ

′ ′ ′ ′ ′

= + − + + − + + − +

′ ′ ′

+ + − + + − −

(16)

The factors in equation (16) can be rearranged in the form

3

0 a b

δ

=

+ which then

yields one unique solution for

3

δ

Ⱐ睨楣栠捡渠瑨敮e畢獴楴畴敤湴漠敱畡瑩≥湳
ㄳ⤠

慮搠⠱㐩⁴漠祩敬搠

2

δ

湤=

1

δ

Ⱐ牥獰散瑩癥汹⸠⁃汥慲汹⁴桥,捯′p汥硩瑹映瑨攠慮慬祳楳i

杲潷猠獵扳瑡湴楡汬礠睩瑨⁴桥摤楴楯=映敡捨 牯=獩湧⁰潩湴⸠⁈潷敶敲⁴桩猠獹獴敭慮=

扥慰楤汹潬癥搠景爠愠牥慳潮慢汥畭b敲e 潦潮瑡捴猠畳楮朠愠oa瑨敭慴楣慬⁰慣a慧攠

睩瑨祭扯汩挠慮bl祳楳a灡扩汩瑹⸠⁔h攠捡e 捵污瑩潮慮攠捨散步搠景爠捯湳楳瑥湣礠批′

獵浭楮朠瑨攠景牣敳牯洠慬氠捯湴慣瑳湤s 捨散歩湧⁴桡琠瑨潳攠景牣敳楶敮礠瑨攠

捡汣′污瑥搠li獰污捥s敮瑳汳漠祩敬搠瑨潳攠摩獰 污捥le湴献†呯敥潷⁴桩n灰汩敳渠

灲慣瑩捥Ⱐ捯ps楤敲⁴桥潬汯睩湧業p 汥慳攠潦慬映晩扲攠潦敮杴栬l L=1000 μm and

a network strain,

ε

Ⱐ潦‰⸰㌮†⁓瑲敳猠楳⁴牡湳晥牲敤,瑯⁴桥慬映晩扲攠慴″≥湴慣瑳琠

( )

1 2 3

,,

x

x x

=

( )

300μm,600μm,900μm

and the normalised stress transfer coefficients

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

are

1 2

10,000

β

β β

′ ′ ′

= = =. Substitution of these values in equation (16) and solving

yields

3

216/91

δ

= − μm, from which

2

45/91

δ

=

− μm and

1

9/91

δ

=

− μm can be

obtained. The correctness of the solution can be shown by substituting these values

into equation (2) which yields

6

1 1

216 45 9

10,000 10 0.03

91

xδ

−

⎛ + + ⎞

⎛ ⎞

= −

⎜ ⎟

⎜ ⎟

⎝ ⎠

⎝ ⎠

which is

0.09890−

μm or -9/91 μm.

The correctness of the solution is proven as equation (2) was not used as part of the

derivation of equation (16).

Applications

There are three major applications for the method. The first application is in

calculating the load distribution in a fibre when the stress transfer varies along the

length of the fibre. This will occur in any nonwoven or nonwoven composite. It will

also occur in composites where stress transfer occurs across the ends of the fibres.

The second application is to model the evolution of the stress development as loading

progresses towards failure and the bonds transferring the load begin to fail. The third

application is to model stress transfer in non-uniform fibres, where elastic modulus

and cross-sectional area vary along the fibre.

To demonstrate the first application, a system is considered with a half fibre of

1000μm length with 20 contacts, at 50μm, 100μm, 150μm…1000μm. Instead of

β

′

=10,000 used in the previous example,

β

′

慳敥渠来湥牡瑥搠慳慮摯=畭扥爠

敩瑨敲整睥敮‰湤‵ⰰ〰
晩扲敳‱ⴳ⤠潲整睥敮‰湤‱〰〠⡦楢牥猠㐭㘩⸠†周攠

牥獵汴猠慲攠獨潷渠楮⁆楧畲攠㌠ 慳⁴桥慴楯映瑨攠汯捡氠獴 牡楮汯湧⁴桥楢牥⁴漠瑨攠

湥瑷潲欠獴牡楮⸠⁁汬瑲慩渠摩 獴物扵瑩s湳牥im楬慲渠獨慰攠瑯⁴桥污獳楣h敡爭污朠

摩獴物扵瑩潮猠瑨敹牥灰牯硩da瑥汹潮≥ 瑡≥≥⁴=睡牤猠瑨攠浩摤汥映瑨攠晩扲攠慴w

0=x

and fall at an increasing rapid rate towards the end of the fibre. The strain at

0x =

for fibres 1-3 is essentially the same as the network strain, while fibres 4-6 with

the lower stress transfer coefficient have a maximum strain of around 0.9 of the

network strain. The random distribution of

β

′

汯湧楢牥慮攠潢獥牶敤猠瑨攠

fa汬渠l≥牡楮潶楮朠瑯睡牤猠瑨攠oib±攠敮搠楳 敩瑨敲⁵湩景牭,潲摥湴楣慬牯=楢牥=

瑯楢牥⸠⁔≥攠晩杵牥桯w猠瑨慴瑲慩渠 摩獴物扵瑩潮猠du捨敳猠摥灥湤敮琠潮⁴桥′

癡汵敳映

β

′

when the values of

β

′

牥楧桥爠潮癥牡来⸠†

=

呯敭潮獴牡瑥⁴桥散潮搠慰灬楣慴楯測o 瑨攠摥扯湤楮朠潦楢牥牯≥潡摥搠

湯湷潶敮瑲畣瑵牥⁷楬氠扥業u污瑥搮†周攠 湯渭睯癥渠瑡步渠慳渠數慭灬攠楳⁰慰敲p

獡sp汥⁴桡琠捯le猠s±潭渠楮癥=瑩条≥楯渠楮 瑯慣瑯牳晦散瑩湧⁴桥瑲敮杴栠潦⁰慰敲≥

⡈攬′〰㔩⸠⁔桥瑡牴楮朠(a瑥物慬⁷慳≥ 湥癥爠扬敡捨敤Ⱐ畮摲楥搬慢潲慴潲礠捯潫敤n

牡摩慴愠灩湥牡晴⁷楴栠愠歡灰愠湵±扥爠潦b ㌰⸠†周楳⁰畬瀠睡猠灲数慲敤牯3⁴桥=

獴慲瑩湧瑯捫礠摯畢汥牡捴楯湡瑩潮渠愠桹摲 潣祣汯湥Ⱐ睨楣栠慬瑥牥搠瑨攠晩扲攠捲潳猭

獥捴楯湡氠獨慰攬⁷桩汥敥灩湧⁴e攠晩扲攠汥湧瑨≥獥湴楡汬礠捯ss瑡湴⸠⁔桥楢牥桡灥≥

睡猠w敡獵牥搠楮⁴桥桥整⁵獩湧e浢 楮慴楯渠潦敳楮i扥摤楮朠慮搠捯湦潣慬b

mi捲潳捯灹
䡥琠慬⸬′〰㌩⸠⁔桥楢牥′ 慰攠aa猠瑨敮桡牡捴敲楳敤礠s敡獵物湧e

瑨攠捲潳猭獥捴楯湡氠慲 敡映瑨攠楲牥杵污爠晩扲攠獨慰攠l 湤牯n⁴桥業e湳楯湳映瑨攠

獭慬汥獴散瑡湧畬慲潵湤楮朠扯砠瑨慴潵a 搠扥楴瑥搠慲潵湤⁴桥楢牥
䡥琠慬⸬d

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

2003). The summary data for the sample are shown in Table 1. The fibre cross-

sectional area was assumed to be constant along the length of the fibre.

The fibre-fibre contacts in the structure were also measured by examining fibres

sectioned longitudinally by the sheet cross-section (He et al., 2004) and directly

counting fibres in contact. The distances between fibre contact centres,

1

n n

x

x

−

−

,

were measured and shown to be fitted by a two-parameter Weibull probability density

function (PDF), as given by equation (17),

( ) ( )

( )

(

)

1

1 1 1

( )/) exp(/

c

c

n n n n n n

c

f

x x x x b x x b

b

−

− − −

− = − − −

(17)

where

b

and

c

are constants, and

,0b c >, and

1

0

n n

x x

−

−

≥. For the sample

simulated here, the fitted parameters were

86.1b

=

µm and

1.43c

=

. Each contact

was assigned to be either a full or a partial contact, depending on whether the entire

width of the fibre was in touch with the fibre of interest or not. Partial contacts arise

because the fibres become twisted during the sheet making process. For the sample

simulated here only 24% of the measured contacts were classified as full contacts.

The contact positions for each fibre were randomly generated from the probability

density function given in equation (17). The distance to the first contact from

0x =

was generated from half the value generated by initial application of equation (17), as

the calculation assumes that the fibre contacts are distributed symmetrically around

the middle of the fibre. The distance to the second contact was then generated from

equation (17) and added to the position of the first contact. Contacts were generated

in this manner until the end of the fibre was reached.

The simulations presented here examined the effect of the randomly assigned

configuration of the crossing fibres. To do this, it was assumed that the stress

transfer coefficient was the same for all fibre contacts at

1000

j

β

′

=

. The orientation

distribution of the crossing fibres was also neglected. Instead it was assumed that

each fibre crossed at the average crossing angle of /2 1

av

θ

π

=

− (He et al., 2003).

Each contact was randomly assigned to be either a full contact or a partial contact,

according to the measured statistics. The area of each full contact was then assumed

to be

2

/sin

w av

D

θ

, where

w

D

is the fibre width shown in Table 1. The area of each

partial contact was randomly assigned a fraction,

λ

Ⱐ扥瑷敥渠〠慮搠ㄠ潦⁴桥牥愠潦,

晵汬潮瑡捴⸠⁆潲⁴桥⁰畲灯獥猠 潦⁴桩猠慮慬祳楳Ⱐ瑨攠獨敡爠扯湤 瑲敮杴栠潦⁴桥潮瑡捴猠

睡猠慳獵we搠瑯攠

b

σ

= MPa such that the breaking load of an individual partial

contact was

2

/sin

b w av

D

λ

σ θ. The possible fracture of the fibres was ignored. The

elastic modulus of the fibres was assumed to be 30 GPa.

For the simulations the network strain was started at 0 and then increased in steps of

0.002 to a final strain of 0.046. For each network strain, the stress distribution along

the fibre and the load at each contact was calculated. The load at an individual

contact was then compared with the breaking load of the contact. If the breaking load

of the contact was exceeded, then the contact was removed from the simulation and

the stress distribution and load at each contact was recalculated. This cycle was

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

repeated until the load at each contact was less than the breaking load of the contact,

after which the network strain was then incremented by 0.002 and the cycle repeated.

The results of the simulation are shown in detail for two fibres in Figures 4 and 5. To

simplify the presentation of the figures only the simulations at strains at intervals of

0.006 have been shown. Fibre 1 (Figure 4) and fibre 2 (Figure 5) have 14 and 25

contacts, respectively. Such a wide distribution of contacts is solely due to the

distribution of distances between contacts given in equation (17). The measured load

distributions along the length of the fibres show similar patterns for both simulations.

No bond breakage occurred for network strains of 0.006, 0.012 and 0.18 for fibre 1. If

there are no bond breakages, then the load distributions will scale with the network

strain, as the fibre is assumed to be linearly elastic. This is observed in Figure 4, in

that the load, at any given position, calculated at a network strain of 0.18 is three

times the load calculated at a network strain of 0.006. In contrast the first bond for

fibre 2 was calculated as breaking at a network strain of only 0.08, despite the

increased number of contacts transferring stress into the fibre. This is due to the area

of this individual contact being particularly small.

It is also interesting to note that the maximum load developed at the middle of fibre 1

at a network strain of 0.006 was 0.0189N, while the corresponding maximum load for

fibre 2 at the same network strain was 0.0248N. The difference between the two was

entirely because the fibre 2 has far more contacts transferring load.

For fibre 1, 1 bond broke at a network strain of 0.02 and a further five bonds broke at

a network strain of 0.022 and the fibre began to debond from the network, so that only

the section of the half fibre between 0 and 600µm was under load at a network strain

of 0.036. This debonding process was accompanied by a sharp drop in the maximum

load on the fibre. For fibre two, five bonds had already broken at a network strain of

0.02 and a further five bonds broke when the network strain was increased to 0.022

and this fibre also began to debond from the network at the end.

Figure 6 shows the fibre average load for six fibres as a function of network strain, as

well as the average of the six fibres. Figures 4 and 5 show the load distribution along

fibres 1 and 2, respectively, from which the fibre average loads were calculated. The

individual fibres, as well as the average curve, all display an initial linear region.

Except for fibre 5, all fibre load-strain curves also display a yield point, occurring

before the point of maximum load. This yield point corresponds to the first bond

failure. The six fibres display wide variability in the maximum load attained and the

strain at the point of maximum load, despite the fact that the individual fibres all have

the same elastic modulus and cross-sectional area and the stress transfer coefficient at

each point of contact is identical. This variability is due only to the distributions in

the number and area of the contact points.

This type of analysis can be used to simulate the failure of paper and other

nonwovens. This is because the failure of paper and other nonwovens is generally

triggered by the failure either by fracture or by debonding of those fibres aligned with

the stress direction. A number of additional factors would need to be considered in

order to do develop an accurate simulation.

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

For nonwovens made of natural wood pulp fibres, variation between and along the

fibres must be taken into account. Elastic modulus in wood pulp fibres varies

systematically with position in the tree (Long et al., 2000) controlled by the

orientation of the cellulose microfibrils with respect to the long axis of the fibre (Page

et al., 1972). Random defects introduced in the pulping process also reduce the

overall elastic modulus measured from single fibre tests (Page et al., 1972), as well as

the elastic modulus at the location of the defect. Further defects are introduced at

fibre-fibre contacts due to differential shrinkage as the fibres dry after the sheet is

formed from fibres in suspension (Page and Tydeman, 1966), producing an area of

lower elastic modulus with low yield stress. Individual wood fibres also have a cross-

sectional area that is approximately constant in the middle of the fibre but tapers to a

point at the fibre’s ends (Cote, 1980). It is not known if local elastic modulus

correlates in any way with local cross-sectional area.

The tapering of the cross-sectional area and variation, from segment to segment, of

elastic modulus along a fibre can be readily modelled using the approach presented

here, as both elastic modulus and cross-sectional area can be set independently for

each segment. The method is also rapid enough to make sufficient simulations for

averages of fibre properties.

One limitation of the method is that it is restricted to linear elastic fibres and the

accuracy of the simulation would need to be carefully considered if significant plastic

deformation of the fibres is expected.

Conclusions

A new method has been developed to calculate the force distribution on a fibre in a

loaded network where force is transferred into the fibre at discrete points. The method

allows for any distribution of contact points and for each contact point to have its own

stress transfer coefficient. The method show great promise in analysing the failure of

nonwovens and nonwoven composites.

Acknowledgements

The support of the Australian Research Council through the Large grant program is

acknowledged. Dr Jihong He is acknowledged for useful discussions.

References

Astrom J., Saarinen S., Niskanen K., Kurkijarvi J., 1994. Microscopic mechanics of

fiber networks. Journal of Applied Physics 75(5), 2383-2392.

Carlsson L.A., Lindstrom T., 2005. A shear-lag approach to the tensile strength of

paper. Composites Science and Technology 65(2), 183-189.

Clyne T.W., 1989. A simple development of the shear lag theory appropriate for

composites with a relatively small modulus mismatch. Materials Science and

Engineering a-Structural Materials Properties Microstructure and Processing 122(2),

183-192.

Cote W.A., 1980. Papermaking fibers : A photomicrographic atlas Syracuse

University Press, Syracuse.

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

Cox H.L., 1952. The elasticity and strength of paper and other fibrous materials.

British Journal of Applied Physics 3(3), 72-79.

Eichhorn S.J., Young R.J., 2003. Deformation micromechanics of natural cellulose

fibre networks and composites. Composites Science and Technology 63(9), 1225-

1230.

Feldman H., Jayaraman K., Kortschot M.T., 1996. A monte carlo simulation of paper

deformation and failure. J. Pulp Pap. Sci. 22(10), J386-J392.

He J., Batchelor W.J., Markowski R., Johnston R.E., 2003. A new approach for

quantitative analysis of paper structure at the fibre level. Appita J. 56(5), 366-370.

He J., Batchelor W.J., Johnston R.E., 2004. A microscopic study of fibre-fibre

contacts in paper. Appita J. 57(4), 292-298.

He J., 2005. Quantitative study of paper structure at the fibre level for the

development of a model for the tensile strength of paper, PhD Thesis. Monash

University, Melbourne.

Long J.M., Conn A.B., Batchelor W.J., Evans R., 2000. Comparison of methods to

measure fibril angle in wood fibres. Appita J. 53(3), 206-209.

Nairn J.A., 1997. On the use of shear-lag methods for analysis of stress transfer

unidirectional composites. Mechanics of Materials 26(2), 63-80.

Page D.H., Tydeman P.A., 1966. Physical processes occurring during the drying

phase, in: Bolam F., (Ed. Consolidation of the paper web transactions of the

symposium held at cambridge, september 1965. Technical Section of the British Paper

and Board Makers' Association, London, pp. 371-396.

Page D.H., El-Hosseiny F., Winkler K., Bain R., 1972. The mechanical properties of

single wood-pulp fibres. Part i: A new approach. Pulp Paper Mag. Can. 73(8), 72-77.

Page D.H., Seth R.S., 1980. The elastic modulus of paper ii. The importance of fiber

modulus, bonding, and fiber length. Tappi 63(6), 113-116.

Raisanen V.I., Alava M.J., Niskanen K.J., Nieminen R.M., 1997. Does the shear-lag

model apply to random fiber networks. Journal of Materials Research 12(10), 2725-

2732.

Sridhar N., Yang Q.D., Cox B.N., 2003. Slip, stick, and reverse slip characteristics

during dynamic fibre pullout. Journal of the Mechanics and Physics of Solids 51(7),

1215-1241.

Xia Z., Okabe T., Curtin W.A., 2002. Shear-lag versus finite element models for

stress transfer in fiber-reinforced composites. Composites Science and Technology

62(9), 1141-1149.

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

Fibre mid-point: x=0 Fibre end: x=L

θ

i

x

1

x

2

x

i-1

x

i

Seg. 1

Fibre mid-point: x=0 Fibre end: x=L

θ

i

x

1

x

2

x

i-1

x

i

Seg. 1

Figure 1 Unstrained half fibre of length,

L

, with

i

crossing fibres.

Seg. 1

1 1

xε

1

xε

1

δ

1

F

Seg. 1

1 1

xε

1

xε

1

δ

1

F

Figure 2. Displacement of the first crossing point from equilibrium position in the

applied strain field,

ε

⸠†

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0.9

1

0 200 400 600 800 1000

Contact position

Local fibre strain/network strain

fibre #1

fibre #2

fibre #3

fibre #4

fibre #5

fibre #6

Figure 3. Calculated stress distributions for six fibres. Fibres 1-3 have

j

β

′

for each

contact having a random value between 0 and 10,000. Fibres 4-6 have

j

β

′

for each

contact having a random value between 0 and 1,000.

0

0.01

0.02

0.03

0.04

0.05

0.06

0 200 400 600 800 1000 1200 1400 1600

Position along fibre (

μ

m)

Load (N)

ε=0.006

ε=0.012

ε=0.018

ε=0.024

ε=0.030

ε=0.036

Figure 4. Load distribution along fibre 1 with 1000

j

β

′

=

and fibre and fibre network

statistics given in Table 1. The legend indicates the overall network strain along the

length of the fibre.

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

0

0.01

0.02

0.03

0.04

0.05

0.06

0.07

0.08

0 200 400 600 800 1000 1200 1400 1600

Position along fibre (μm)

Force (N)

ε=0.006

ε=0.012

ε=0.018

ε=0.024

ε=0.030

ε=0.036

Figure 5. Load distribution along fibre 2 with 1000

j

β

′

=

and fibre and fibre network

statistics given in Table 1. The legend indicates the overall network strain along the

length of the fibre.

0

0.01

0.02

0.03

0.04

0.05

0.06

0.07

0.08

0.09

0.1

0 0.01 0.02 0.03 0.04 0.05

Network strain

Average force along fibre (N)

Fibre 1

Fibre 2

Fibre 3

Fibre 4

Fibre 5

Fibre 6

Average of fibres 1-6

Figure 6. Simulations of average force along the fibre versus network strain for six

fibres.

Preprint of article appearing in Mechanics of Materials vol 40 (12) p 975-981 and

available at doi:10.1016/j.mechmat.2008.07.003

Table 1 Fibre and sheet parameters for the material used in the simulations.

Pulp Hydrocyclone Fraction Sheet Pressing level

Radiata pine, Kappa

number of 30

Reject 0 MPa

Fibre height (μm) Fibre width (μm) Fibre wall area (μm

2

)

16.45

±

0.93 30.19

±

ㄮ㌵‱㤲

±

10

Fibre length

No. of full contacts per fibre

(average)

No. of partial contacts per

fibre (average)

3.34 mm 10.6 32.9

Sheet apparent

density (kg/m

3

)

Length weighted Fibre

length (mm)

218 3.14

## Σχόλια 0

Συνδεθείτε για να κοινοποιήσετε σχόλιο